Microstructure and luminescence dynamics of ZnCdO films...
Embed Size (px)
Transcript of Microstructure and luminescence dynamics of ZnCdO films...
Microstructure and luminescence dynamics of
ZnCdO films with high Cd content deposited on
different substrates by DC magnetron
I. Shtepliuka, Volodymyr Khranovskyy, G. Lashkarev, V. Khomyak, A. Ievtushenko, V.
Tkach, V. Lazorenko, I. Timofeeva and Rositsa Yakimova
Linköping University Post Print
N.B.: When citing this work, cite the original article.
I. Shtepliuka, Volodymyr Khranovskyy, G. Lashkarev, V. Khomyak, A. Ievtushenko, V.
Tkach, V. Lazorenko, I. Timofeeva and Rositsa Yakimova, Microstructure and luminescence
dynamics of ZnCdO films with high Cd content deposited on different substrates by DC
magnetron sputtering method, 2013, Applied Surface Science.
Postprint available at: Linköping University Electronic Press
Microstructure and luminescence dynamics of ZnCdO films with high Cd
content deposited on different substrates by DC magnetron sputtering
I. Shtepliuk1, V. Khranovskyy2, G. Lashkarev1, V. Khomyak3, A. Ievtushenko1,
V. Tkach4, V. Lazorenko1, I. Timofeeva1, and R. Yakimova2
1Institute for Problems of Material Science, National Academy of Sciences of Ukraine, Kiev
2Linköping University, Department of Physics, Chemistry and Biology, Linköping 58381, Sweden
3Chernivtsi National University, Chernivtsi 58012, Ukraine
4Bakul Institute for Superhard Materials, National Academy of Sciences of Ukraine, Kiev 04074,
Investigation of Cd behaviour in the ZnCdO alloys, where Cd content exceeds the solubility limit, is
of importance due to possible impurity segregation and second phases’ formation in this material.
We have studied the Cd behaviour in the Zn1-xCdxO films deposited by dc magnetron sputtering on
different substrates: c-plane Al2O3, bare Si (100) and Au (45 nm)/Si (100). It is revealed that Cd
content of 10 at. % in the target results in average 6 – 8 at. % of Cd in the films, depending on the
substrate type. Structural analysis based on x-ray diffraction revealed the absence of Cd-related
secondary phases. Time-resolved photoluminescence (TRPL) and high-resolution energy dispersive
X-ray analysis (EDX) help to understand the recombination dynamics of spontaneous emission and
to establish correlations between cadmium content and radiative lifetime. We have revealed that the
internal quantum efficiency is influenced by the Cd content and defect concentration. It is suggested
that increasing of the cadmium content results in the reduction of nonradiative recombination
centers originating from point defects.
Key words: ZnCdO, growth kinetics, lattice defects, photoluminescence, substrate
ZnO has been recognized as a material of paramount importance for fabricating optoelectronic
devices operating in the blue/UV region [1 - 10]. This is due to a combination of its specific
semiconductor and material properties. It has a wide direct band gap of 3.36 eV at room
temperature, which can be modified in a wide range via alloying with Cd (down to 2.8 eV) or Mg
(up to 4.0 eV) . The exciton binding energy is around 60 meV at room temperature, which is one
of the highest among other optoelectronic materials. It should be noted that the band-gap
engineering for ZnO is vital for its further progress in optoelectronics: isoelectronic cadmium
impurity is an ideal candidate for reducing the band gap of zinc oxide . ZnCdO solid solution has
the advantage of tunability of the alloy band gap, allowing larger control over the spectrum of
emitted light from near UV to visible [4, 5]. Many interesting phenomena like tunable
electroluminescence from n-ZnCdO/p-GaN heterojunction , luminescence enhancement effect of
deuterium in ZnO/ZnCdO quantum wells , enhancement of the spontaneous emission rate from
ZnCdO quantum wells by surface plasmon coupling , rectifying behavior of a p–n junction based
on n-Zn0.94Cd0.06O/p-SiC heterostructures  and effect of transparent thin film transistor based on
ZnCdO  have already been reported. However, many fundamental optical properties of ZnCdO
have not been extensively studied. The dynamic behavior of the carriers in the ZnCdO solid
solutions is not yet fully understood and is still controversial. Yamamoto et. al  reported that
the PL lifetime of ZnO (125 ps) gradually increases with increasing Cd content under 0.19,
showing a typical slow PL lifetime of 125 ps. At Cd content over 0.3, it drastically increased up to
54 ns and was two orders longer than that in ZnO . The decay times τ1 and τ2 for the excitons at
8 K were 16 and 80 ps, respectively, in Zn0.85Cd0.15O grown by remote-plasma enhanced
metalorganic chemical vapor deposition . However, the exciton at 2 K has the radiative lifetime
of 3 ns in the Zn0.843Cd0.157O grown by molecular-beam epitaxy .This large discrepancy of
lifetimes is closely related to the crystalline quality and the photoluminescence center is very
sensitive to the micro-structure. Therefore, this useful information of TRPL dependency on the
crystalline quality can be extended into the optimization of the growth conditions of the ZnCdO
solid solution. Thus, it is important to understand the fundamental properties of the optical process
and emission mechanism in ZnCdO alloys depending on Cd content and growth parameters (for
example, a substrate type), especially for Cd-rich ZnCdO alloys for further improvement of
Earlier, ZnCdO films grown on different substrates, such as indium tin oxide (ITO) ,
sapphire , Si , quartz  and glass  have already been studied. For example, Ma et. al
 have shown that the type of substrate significantly influences the structure, morphology and the
transmittance of the Zn1-xCdxO films. It was demonstrated that the Zn0.8Cd0.2O/a-Al2O3 film had a
better crystal quality than that on the Si substrate. Additionally, there was a difference of the band
gap energies between the samples which were deposited on the glass and a-sapphire substrates. It
was explained that the ions coalesce more tightly in the Zn0.8Cd0.2O/a-Al2O3 film and the evaluated
band-gap-energy was larger. Moreover, Fouzri et al.  have revealed that the substrate
orientation significantly influences the Cd incorporation in ZnCdO. Nevertheless, the substrate
effect on the structural and optical features of ZnCdO films is not fully understood, and requires
further investigations. Clear understanding of the substrate effect is valuable for potential
applications of ZnCdO ternary alloy and respective device fabrication since the kind of the growth
surface determines the device performance.
In this work, we report structural and luminescence properties of ZnCdO films produced by
direct current (DC) magnetron sputtering on different substrates: bare and Au-coated (30 nm) Si
(100) and c-Al2O3 (0001). Assuming that the solubility limits may be influenced by the tensile
strain in the films, we have chosen the substrates that provide in-plane tensile strain for ZnCdO
growth. We also present results of the time-resolved photoluminescence (TR PL) measurement of
the ZnCdO layers at room temperature. Our experimental data strongly support the hypothesis that
the substrate type may considerably influence the PL dynamics, equilibrium cadmium content and
microstructure of the ZnCdO ternary alloys.
2. Experimental details
The films of Zn1-xCdxO ternary alloy were deposited on Au/Si (100), Si (100) and c-Al2O3 (0001)
substrates at the temperature of 400 °C by direct current magnetron sputtering. A disc of zinc-
cadmium alloy (100 mm in a diameter) with a purity of 99.99% was used as a target. High purity
argon and oxygen gases were used as the sputtering and the reactive gas, respectively. The target-
to-substrate distance was 40 mm. The chamber was pumped to a base pressure of 1·10-4 Pa before
deposition. The films were grown in the ambient with Ar/O2 ratio of 4:1. The dc power was
maintained at 150 W. The deposition time was 60 min for all samples. The crystal structure of the
samples was studied by the XRD analysis where the CuKα1 radiation was used as a source (λ =
0.154056 nm). The XRD measurements were carried out by the DRON-4 Powder Diffraction
system; a scan rate of 1°/min and a step size of 0.01° were used. It is important to note that the
analysed surface is about ~1 cm2 and the penetration depth of X-rays at 20–40 keV is a few
microns. Measurement error of the peak position is about ± 0.01°(2θ). Error of the c-lattice
parameter is about ± 0.0003 nm. The relative error in the FWHM has been estimated to be ± 2%.
Time-resolved PL (TR PL) measurements were performed by means of a third harmonic of a
femtosecond pulsed Ti:sapphire laser mode-locked laser with a repetition frequency of 75 MHz set
at 266 nm as an excitation source. The resulting PL was recorded by a streak camera system with a
time resolution of ~ 8 ps. Scanning electron microscopy (SEM) was used to reveal the uniformity of
the films (ZEISS EVO 50 XVP). An acceleration voltage was fixed at 20 kV. An elemental analysis
of the ZnCdO films were also done by ZEISS EVO 50 XVP SEM using energy dispersive X-ray
spectroscopy (EDX) furnished INCA 450 (OXFORD Instruments). The atomic concentrations of
Zn, Cd and O elements were determined within the relative experimental error of ~2%. An
operating voltage for EDX analysis was set to 20 kV. The area of 500 µm x 500 µm was studied to
determine the concentrations of the elements. The thickness of the films was ~1.5 µm for all
samples, determined from the SEM images of the cross section of the films (not shown in the
3. Results and discussions
In the case of heteroepitaxial growth, substrate influences the structural parameters of the
overgrown material due to lattice and thermal expansion coefficient (TEC) mismatch [20, 21].
Table 1 represents the structural parameters of the ZnO in comparison to silicon and sapphire
The properties of ZnO, Si and Al2O3
Parameter ZnO Si Al2O3 Eg (eV) 3.34a 1.12d 8.8e
Lattice constant (Å) a=3.250b c=5.205b
a=5.43f a=4.758h c=12.992h
Coefficient of Thermal expansion (10-6 K)
2.9c 2.6f 7.5c
aRef.. bRef.. cRef.. dRef.. fRef.. eRef.. hRef..
Fig. 1 illustrates the θ-2θ XRD patterns of Zn1-xCdxO films grown on different substrates,
confirming that the Zn1-xCdxO ternary alloys possess a hexagonal wurtzite structure. All deposited
films have a polycrystalline structure with strong (002) preferred orientation. The relative intensity
of the (002) diffraction peak provides further evidence that the films are preferentially oriented in
the c-axis direction.
Fig. 1 XRD patterns of Zn1-xCdxO films grown on (a) Au-coated Si, (b) Si and (c) c-Al2O3
The growth of the ZnO film along the (002) direction is due to the lowest surface free energy of the
(002) plane of ZnO . The XRD θ-2θ scan of ZnCdO films, grown on Au coated Si substrate,
revealed only peak due to the reflections from (002) plane of ZnO (Fig. 1a). Only ZnO wurtzite
phase, therefore, is detected and no evidence of other phases was observed. Similarly, the film on a
bare Si substrate displayed only the (002) reflection peak (Fig. 1b).
In both cases the substrate peaks are also visible, thereby indicating a rather small thickness of the
films. While the ZnCdO films, grown on sapphire, are characterized by the additional weak peaks
of (110) and (211), as shown in Figure 1c. Such a feature may be explained in terms of the high
lattice mismatch between (0001) sapphire and (0001) ZnO (Table 1), which can promote the lattice
disorder, reorientation of the crystallites and appearance of the new diffraction peaks. In order to
confirm this assumption we have calculated the Lotgering factor  for different samples and have
found that the sample grown on the sapphire exhibit Lotgering factor of ~0.75. Whereas the
samples grown on the Si and Au-coated Si demonstrate the higher degree of orientation of the
ZnCdO films along the c-axis (Lotgering factor ~1). It should be noted that no reflexes
corresponding to the separate CdO phase or metallic Cd clusters are observed. It may be caused by
two factors: (i) XRD method is not sensitive enough and possible formation of the second phases
could not be observed and (ii) in the case of non-equilibrium growth conditions, the level of Cd
incorporation may exceed the Cd solubility limit in ZnO, which was theoretically suggested 2 % by
the Brown et. al. . We assume that in our case we have a fluctuation of Cd content and possible
segregation of the dopant on the grain boundaries, film/substrate interface etc. Nevertheless, part of
Cd ions incorporates into ZnO lattice. In order to investigate this assumption, we performed a
comparative analysis of XRD (002) peaks appertaining to Zn1-xCdxO films grown on the different
substrates. A vertical line (Fig. 2) in this figure corresponds to the standard (002) reflex of ZnO
wurtzite structure accordingly to JCPDS card 36-1451 . Here we have to be aware that in our
case several different factors may effect on the (002) peak position: i) substrate lattice mismatch ii)
TEC mismatch between substrate and film iii) Cd incorporation. Interestingly, these factors are
commonly interrelated and complementary. A certain type of the substrate, depending on the
provided in-plane strain – tensile or compressive, may promote or prevent the impurity
incorporation. Earlier, it was reported, that the tensile in plane stress favours Ga incorporation into
ZnO . Our XRD data, obtained for films on different substrates but at the same Cd content in
the target, clarify these issues as following. Both lattice mismatch between Si and ZnO (~40% )
and Al2O3 and ZnO (18% or 31.8% in the case of in-plane twist at high temperature growth )
are rather significant.
Fig. 2 XRD patterns in the 2θ range of 33°-37° of Zn1-xCdxO films grown on three substrates: (a)
Au-coated Si, (b) p-Si and (c) c-Al2O3. On the top of the image the respective effect of lattice
mismatch and Cd incorporation effect on position of (002) peak is shown. The vertical line is a
position of (002) peak for strain free ZnO.
However, as a result of used growth techniques, the obtained films are polycrystalline, which by-
turn leads to mitigation of the lattice mismatch by large extent. Therefore, we claim that in our case
Cd incorporation by itself is most influential factor on the structural characteristics of the ZnO
films. Due to the Cd and Zn ionic radii - 0.97 Å in comparison to 0.74 Å, when Cd substitutes Zn in
his lattice sites, both a and c lattice parameters are enlarged. For the hexagonal lattice the position
of the (002) reflection is directly related to the c-lattice parameter via the diffraction angle as
where λ is the CuKα1 radiation, and θ is the diffraction angle. Thus, the Cd incorporation should
increase the c value. While in the case of epitaxial growth both substrates should decrease the c-
lattice parameter (due to expected tensile in-plane stress ) and thus, the (002) peak should occur
toward the higher diffraction angles. However, as one can see, in our case for Si and Au/Si
substrates, the (002) peaks are shifted toward smaller diffraction angles, thereby evidencing the
increase of c-parameter (Fig. 2). This increase of c-lattice parameter is associated with Cd
incorporation and is agreed in a previous report . However, the substrate by itself affects the
average Cd content. While for the case of sapphire substrate, the effect of substrate (lattice
mismatch (LM) effect) is more influential. Apparently, the (002) peak has been initially shifted
toward higher diffraction angles. It is owing to tensile in plane strain provided by the substrate. And
afterwards - being compensated by Cd incorporation - it underwent the shift toward opposite
direction. It is generally known that the considerable difference in the lattice periods between the
film and the substrate will lead to an appearance of compressive stresses. ZnO films grown on c-
Al2O3 substrates always undergo serious residual strain induced by the lattice mismatch
[aAl2O3−aZnO] /aAl2O3=−18.3%  and the difference of coefficient of thermal expansion (CTE):
[CTEAl2O3−CTEZnO]/CTEAl2O3=−34% . Cadmium incorporation will lead to the lattice
expansion and will cause the appearance of the tensile stresses. It is due to the difference in ionic
radii between zinc and cadmium . Therefore, the (002) peak of the ZnO, which is grown on the
sapphire, is always shifted towards the side of larger Bragg angles due to the compressive stresses.
When the solid solution is formed, the (002) peak will displace towards the side of the smaller
Bragg angles due to the compensation effect of the residual compressive stresses by the tensile
stresses. Fig. 2 also demonstrates the value of the FWHM (full width on half maximum) for films
grown on the different substrates. It was revealed that different samples have different values of
FWHM. It may be explained as follows. It is well known that the broadening of the 002 peak is
produced by either lattice strains alone, or by lattice strains and small particle size simultaneously
. Therefore, the different values of the FWHM for different samples are associated with the
individual features of the substrate (lattice and/or TCE mismatch with film, individual rate of
surface diffusion process, thermal conductivity), which can promote (i) growth of large or small
grains and (ii) appearance of tensile (or compressive) strain. That’s why; the films deposited on
different substrates demonstrate different FWHM values.
On the other hand, different compositional fluctuations in the samples can also be a reason for
difference in FWHM values. In fact, it is very difficult to choose a dominant factor. There are
several competing and complementary mechanisms.
Fig. 3 EDX spectrum of the ZnCdO film grown on Au-coated Si.
Moreover, the spectral location of the peak was found to be in correlation with the Cd
content, determined by EDX analysis (Table 2). Thus, we can pre-conclude, that the Cd
incorporation effect is dominant on the lattice parameters of ZnO. Fig. 3 demonstrates the typical
EDX spectrum of the ZnCdO/Au-coated Si, which reveals that the sample is composed of O, Zn,
Atomic content of zinc, cadmium and oxygen for ZnCdO films deposited on different substrates as
well as microstructure parameters of the ZnCdO ternary alloys deposited on the different substrates
Atomic content of elements with errors, at.%
Crystallite size D, nm
O Zn Cd ZnCdO/Au/Si 52±1 42±1 6±0.1 1.08 5.215 +1.84 19
ZnCdO/c-Al2O3 48±1 47±1 5±0.1 0.92 5.199 -1.23 18 ZnCdO/Si 51±1 40±1 8±0.1 1.04 5.277 +13.7 21
A simultaneous influence of both Cd incorporation and substrate type on the crystal lattice leads to
the strain along c-axis in ZnCdO films. The strain value can be estimated by following formula:
ε= (сfilm-сbulk)/сbulk, where сbulk=5.2054 nm. Crystallite sizes were calculated by the Debye-Scherrer
Lattice parameters, crystallites sizes, and strain values determined from the XRD data of all
samples are also presented in Table 2. As one can see from the Table 2, a clear correlation exists
between the atomic content of Cd and the c-lattice parameter. The different cadmium content of the
resultant films on Au-coated Si, bare Si and sapphire may be related to the lattice structure and
defects on the substrate surface, which is an important factor, governing the chemically adsorption
and subsequent nucleation and growth . We supposed that the highest Cd incorporation (8.61
at.%), observed for Zn1-xCdxO grown on Si substrate, may be associated with the fact that the
thermal conductivity of Si is better than that of sapphire. Wei et al.  have revealed that the
difference in thermal conductivity may be a possible reason that the best growth temperature
(400 ◦C) of ZnO thin film fabricated on Si substrate is lower than that of sapphire (500 °C). Since
the growth procedure in our experiment was realized at the substrate temperature of 400 °C then the
Cd incorporation is favored in the Si substrate.
Fig. 4 SEM images of the ZnCdO films grown on the various substrates: (a)Au-coated Si, (b) c-
Al2O3 and (c) Si
The microstructural properties of ZnCdO films deposited on different substrates are shown
in Fig. 4. The films in general demonstrate the microstructure, peculiar for sputtered films – dense
coverage of grains, which are not hexagonally faceted - which is probably due to high deposition
rate and low growth temperature. For all the films rather rough surface was observed. The film,
deposited on sapphire, is slightly different in comparison to others: the grains are better resolved
and can be identified more clearly. This is correlated with XRD and EDX results, which revealed
that the film grown on Al2O3 is characterized by smallest value of the strain and smallest cadmium
content in comparison to other films. The observed rough morphology of the films may be vital for
their application as a top layer for the solar cells. Particularly, surface morphology is an important
characteristic of ZnO films within such area of application as silicon thin film solar cells. It should
be noted that the developed surface texture is required to provide light scattering and subsequent
light trapping inside the silicon solar cell structure .
The possible difference in structural properties between samples grown on Au-coated Si, Si
and sapphire substrates may be explained by the fact that the every substrate associated with an
individual rate of surface diffusion process. It is well known that the mass transport may occur
during crystal growth through surface diffusion process of the adatoms, which is governed by
surface kinetics and is strongly dependent on substrate types . So, we have concluded that the
Au-coated Si, Si and sapphire substrates are characterized by the different values of the time which
described a duration the adatoms undergoes in the diffusion process. In other words, this time may
be the time the adatoms spend on the surface either before being captured in the lattice site or
desorbed from the surface . Apparently, the desorption processes of the Cd adatoms are most
intense for the film which was condensed on the sapphire substrate. In particular, it agrees well with
EDX results. The newly arrived Cd species have no time in order to take place the thermodynamic
lattice sites, thereby promoting the cadmium accumulation at the grain boundaries .
Fig. 5 The PL dynamics of the ZnCdO/ Al2O3 sample: time resolved PL image (a), taken for the
spectral range (b) and the decay time curve (c), fitted respectively.
In order to gain insight into the origin of the radiative recombination, we have performed
time-resolved PL measurements (TRPL) of the samples ZnCdO/Au/Si, ZnCdO/Si and
ZnCdO/Al2O3 at room temperatures. The time decay has been studied integrated for the band as
wide as 380 ÷ 430 nm. Figure 5, for example, demonstrates the PL dynamics of the ZnCdO/ Al2O3
sample: time resolved PL image (a), taken for the spectral range (b) and the decay time curve (c),
fitted respectively. The decaying part of the TRPL data was well described by the bi-exponential
decay function: I(t)=А1exp(-t/τ1)+A2exp(-t/τ2) . Thus, analysis of the decay curves by means of
the mentioned function gives a possibility to extract time constants τ1 and τ2 depending on the Cd
content, which defines by the substrate type (as shown in Table 2). It should be mentioned that the
decay time constants are different for the studied samples.
The sample on sapphire demonstrated the decay time constants τ1 ~ 9 ps and τ2 = 121 ± 18
ps. For the sample of ZnCdO on bare Si τ1 = 30 ± 9 ps (depending on the position on the sample),
while τ2 = 220 ± 20 ps. While for the sample ZnCdO on Au/Si substrate, the τ1 = 29 ± 10 ps and τ2 =
240 ± 45 ps. These time constants are comparable to those of ZnCdO reported earlier by Yang et al.
. An initial fast decay component τ1=τNR is attributed to the capture of excitons and trapping of
carriers by deep centers of defects and impurities (centers of the non-radiative recombination) and
process of the multiphonon emission . A slow decay component τ2=τR describes the lifetime of
radiative recombination for both free and localized excitons . The exciton recombination time at
RT is most likely determined by nonradiative recombination as the obtained values are comparable
to the free exciton lifetime (0.03–0.11 ns) measured at RT from ZnO epilayers but are substantially
shorter than that for bulk ZnO ( ~ 1 ns) with low defect density . For ZnO thin films, earlier it
was shown that the bound exciton decay time is dependent on the grain size and it varied from
47 ps for 40 nm grains to 216 ps for 200 nm grains . Thus, the difference in our case between
samples grown on Si and sapphire substrates may be explained as due to that. Interesting is the
observed effect of Au on the decay time of ZnCdO samples, grown on Au coated Si substrate.
Earlier, Au has been reported responsible for passivation of the non-radiative recombination centers
in ZnO, increasing the decay time significantly. Yang et al. has reported that that the Au particles
can greatly reduce the nonradiative recombination rate by passivation of surface states and make the
decay time slow down . Additionally, we can find the internal quantum efficiency of ZnCdO
ηint(ZnCdО), which can be described as: ηint=(1/ τR)/[(1/ τR)+(1/ τNR)] . Calculated parameters
are shown in the Table 3.
It should be noted that we found a correlation between the Cd content and quantum
efficiency (as shown in Table 3). The film with the largest cadmium content demonstrates the
largest value of the internal quantum efficiency. It may be caused by several factors: (і) decrease in
the concentration of the intrinsic point defects, which may play a role of the non-radiative
recombination centers and (іі) strong exciton localization, which can be a reason for the
enhancement of the probability of the radiative transitions .
Parameters extracted from TRPL data and value of deviation from stoichiometric ratio Parameters Substrate type
c-Al2O3 Si Au/Si τ1=τNR 9 30 29
τ2=τR 121 220 240
Internal quantum efficiency η 0.069 0.119 0.107
Cd content, at.% 5±0.1 8±0.1 6±0.1
Deviation from the stoichiometry, ∆S -0.08 0.04 0.08
Taking into account the first factor (i), we have found a principle relationship between the value of
the deviation of the stoichiometric ratio ∆S, which may be expressed as: ∆S =nO/(nZn+nCd) – 1, and
cadmium content in the film (Fig. 6). The film with the smallest cadmium content (5.1 at. %) is
characterized by the negative magnitude ∆S of -0.08 (conditions of the oxygen deficiency). In these
non-equilibrium conditions, the intrinsic point defects associated with zinc excess, i.e., oxygen
vacancies (VO) and zinc interstitials (Zni), are lowered in formation energy . On the other hand,
the film with the largest cadmium content (8.6 at. %) demonstrates a positive magnitude of the ∆S
value of +0.04 (conditions of the zinc deficiency). In this case, the point defects related to oxygen
excess, i.e., zinc vacancies (VZn) and oxygen interstitials (Oi), are lowered in formation energy .
Thus, the Zn-rich conditions and/or O-rich conditions cause the lowering of the formation energy
EF of the corresponding defects and lead to an increase in the concentration of the corresponding
intrinsic point defects. This statement is thoroughly valid, since the concentration of defects in a
crystal depends upon its formation energy EF in the following form :
where Nsites is the concentration of sites in the crystal where the defect can occur. Therefore, a high
magnitude of the deviation from the stoichiometry implies the low formation energy and the high
equilibrium concentration of the defects. In this case, the role of the non-radiative recombination
processes starts to increase.
Fig. 6. Dependencies of the internal quantum efficiency (circles) and the value of the deviation from
stoichiometric ratio (squares) on the cadmium content.
On the other hand, high formation energy means that the defects are unlikely to form. According to
above-mentioned explanation the increase in Cd content leads to a reduction of the defect
concentration. It is very strange. Nevertheless, we should take into account the fact that the
cadmium ions, incorporating into ZnO matrix, may influence the energetics of the native defects in
ZnO and may either lower the formation energy of the defects or raise the value of EF depending on
the deficiency (or enrichment) of the host atoms. Furthermore, in a previous work , which was
devoted to InGaN (semiconductor analogue of ZnCdO), it was shown that the indium may
sufficiently reduce the density of the non-radiative recombination centers Nt, thereby decreasing
the probability of the non-radiative optical transitions 1/τnon-rad. Physical relationship between
mentioned parameters may be expressed by means of the following formula :
where Vth is the thermal velocity, σ is the cross section captured by the non-radiative recombination
center. Thus, Nt value was greatly suppressed by the addition of a small amount of In . A
similar mechanism of the passivation of the point defects may be also realized in ZnCdO
semiconductor system. However, this assumption requires the additional experimental support.
Taking into account the second factor of the influence – (іі) strong exciton localization – on
the internal quantum efficiency of ZnCdO, it should be mentioned that the increase in Cd content
may cause the large composition fluctuations (large localization depth) and may lead to appearance
of the great number of potential minima, which could capture the excitons, thereby increasing the
probability of the processes of radiative annihilation and blocking the nonradiative optical
transitions. Indeed, it was previously reported [54-56] that the effect of the exciton localization
induced by compositional fluctuation of In leads to the hindering the pathways of nonradiative
recombination centers and capturing the excitons at potential minima. Thus, we have revealed that
the internal quantum efficiency are influenced by the Cd content and defect concentration, which
are depending on the type of the substrate.
In summary, we have studied the microstructure and dynamics of luminescence of Zn1-xCdxO films,
with the Cd concentration over the solubility limit, deposited by dc MS on different substrates. It
was shown that the Cd content has dominant effect on the structural properties of ZnO in terms of
lattice parameters and available strains. However, the type of the substrate does affect the average
Cd incorporation into ZnO films. It was found that the luminescence kinetics of Zn1-xCdxO films
was strongly dependent upon the substrate type and cadmium content and was well described by a
bi-exponential. The occurrence of bi-exponential kinetics leads to the presence of the different
mechanisms for excitonic recombination. We showed using time-resolved photoluminescence
measurements that the internal quantum efficiency increases with increasing the cadmium content
in the solid solution. We explained this behavior in the context of strong exciton localization as well
as blocking the pathways of nonradiative recombination centers. This effect may be useful for the
enhancement of the emission efficiency of the ZnCdO solid solution due to limitation of exciton
movement and increasing the probability of the radiative optical transitions. The reported data
contribute significantly towards understanding the band engineering of ZnO toward visible range or
design of quantum wells heterostructures based on ZnCdO.
We greatly acknowledge the Linköping Linnaeus initiative for Novel Functional Materials (LiLi-
IFM) for the support of this work.
 G. V. Lashkarev, V. A. Karpyna, V. I. Lazorenko, A. I. Ievtushenko, I. I. Shtepliuk and V. D.
Khranovskyy, Properties of zinc oxide at low and moderate temperatures, Low Temp. Phys. 37
 Ü.Özgür, Ya. I. Alivov, C. Liu, A.Teke, M. A. Reshchikov, S. Doğan, V. Avrutin, S.-J. Cho,
H. Morkoç, A comprehensive review of ZnO materials and devices, J. Appl. Phys. 98 (2005)
 F. Wang, Z. Ye, D. Ma, L. Zhu, F. Zhuge, Formation of quasi-aligned ZnCdO nanorods and
nanoneedles, J. Cryst. Growth 283 (2005) 373–377.
 I. Shtepliuk, G. Lashkarev, V. Khomyak, O. Lytvyn, P. Marianchuk, I. Timofeeva, A.
Ievtushenko, V. Lazorenko, Features of the influence of the deposition power and Ar/O2 gas ratio
on the microstructure and optical properties of the Zn0.9Cd0.1O films, Thin Solid Films 520 (2012)
 T. Makino, Y. Segawa, M. Kawasaki, A. Ohtomo, R. Shiroki, K. Tamura, T. Yasuda, and H.
Koinuma, Band gap engineering based on MgxZn1−xO and CdyZn1−yO ternary alloy films, Appl.
Phys. Lett. 78 (2001) 1237–1239.
 F. Fang, D. Zhao, X. Fang, J. Li, Z. Wei, S. Wang, Jilong Wu, D. Shen, X. Wang, Tunable
electroluminescence from n-ZnCdO/p-GaN heterojunction, J. Phys. Chem. Solids 73 (2012) 217–
 W. Lim, D. P. Norton, S. J. Pearton, X. J. Wang, W. M. Chen, A. Buyanova, A. Osinsky, J. W.
Dong, B. Hertog, A. V. Thompson, W. V. Schoenfeld, Y. L. Wang and F. Ren, Migration and
luminescence enhancement effects of deuterium in ZnO/ZnCdO quantum wells, Appl. Phys. Lett.
92 (2008) 032103.
 B. Liu, C. W. Cheng, R. Chen, S. A. Ekahana, W. F. Yang, S. J. Wang, T. C. Sum, Z. X. Shen,
H. J. Fan, and H. D. Sun, Surface plasmon induced exciton redistribution in ZnCdO/ZnO coaxial
multiquantum-well nanowires, Appl. Phys. Lett. 97 (2010) 081107-3.
 I. Shtepliuk, V. Khranovskyy, G. Lashkarev, V. Khomyak, V. Lazorenko, A. Ievtushenko, M.
Syväjärvi, V. Jokubavicius and R. Yakimova, Electrical properties of n-Zn0.94Cd0.06O/p-SiC
heterostructures, Solid-state electron. 81 (2013) 72-77.
 D.-H. Lee, S. Kim, S. Y. Lee, Zinc cadmium oxide thin film transistors fabricated at room
temperature, Thin Solid Films 519 (2011) 4361–4365
 K. Yamamoto, T. Tsuboi, T. Ohashi, T. Tawara, H. Gotoh, A. Nakamura, J. Temmyo,
Structural and optical properties of Zn(Mg,Cd)O alloy films grown by remote-plasma-enhanced
MOCVD, J. Cryst. Growth. 312 (2010) 1703–1708.
 K. Yamamoto, M. Adachi, T.Tawara, H. Gotoh, A. Nakamura, J. Temmyo, Synthesis and
characterization of ZnCdO/ZnO multiple quantum wells by remote-plasma-enhanced MOCVD, J.
Cryst. Growth 312 (2010) 1496–1499
 I. A. Buyanova, J. P. Bergman, G. Pozina, W. M. Chen, S. Rawal, Mechanism for radiative
recombination in ZnCdO alloys, Appl. Phys. Lett. 90 (2007) 261907-3.
 T. Singh, D.K. Pandya, R. Singh, Synthesis of cadmium oxide doped ZnO nanostructures using
electrochemical deposition, J. Alloys Compd. 509 (2011) 5095–5098.
 A. Fouzri, V.Sallet, M.Oumezzine A comparative structure and morphology study of Zn(1-
x)CdxO solid solution grown on ZnO and different sapphire orientations, J. Cryst. Growth 331
 A. Singh, D. Kumar, P.K. Khanna, B. Chander Joshi, M. Kumar, Effect of post annealing
temperature on structural and optical properties of ZnCdO thin films deposited by sol–gel method,
Appl. Surf. Sci. 258 (2011) 1881– 1887.
 B.J. Zheng, J.S. Lian, L. Zhao, Q. Jiang, Structural, optical and electrical properties of
Zn1−xCdxO thin films prepared by PLD, Appl. Surf. Sci. 257 (2011) 5657–5662.
 F. Yakuphanoglu, S. Ilican, M. Caglar, Ya. Caglar, Microstructure and electro-optical
properties of sol-gel derived Cd-doped ZnO films, Superlattices Microstruct. 47 (2010) 732-743.
 D.W. Ma, Z.Z. Ye, Y.S. Yang, A comparative study on Zn0.8Cd0.2O films deposited on
different substrates, Appl. Surf. Sci. 252 (2006) 5051–5056
 R.J. Kennedy, P.A. Stampe, The influence of lattice mismatch and film thickness on the
growth of TiO2 on LaAlO3 and SrTiO3 substrates, Journal of Crystal Growth 252 (2003) 333–342.
 Y.-C. Lee, S.-Y. Hu, W. Water, K.-K. Tiong, Z.-C. Feng, Y.-T. Chen, J.-C. Huang, J.-W. Lee,
C.-C. Huang, J.-L. Shen, M.-H. Cheng, Rapid thermal annealing effects on the structural and optical
properties of ZnO films deposited on Si substrates, J. Lumin., 129 (2009) 148–152
 Cole W. Litton, Donald C. Reynolds, Thomas C. Collins, Zinc oxide materials for electronic
and optoelectronic device applications, Wiley, West Sussex, 2011, p.224.
 S. M. Sze, The Physics of Semiconductor Devices, Wiley, New York, 1969, pp. 12-20.
 R. Hull, Properties of Crystalline Silicon, INSPEC, London, 1999.
 A. O’Mahony, S. Monaghan, G. Provenzano, I. M. Povey, M. G. Nolan, É. O’Connor, K.
Cherkaoui, S. B. Newcomb, F. Crupi, P. K. Hurley, and M. E. Pemble, Structural and electrical
analysis of the atomic layer deposition of HfO2 /n-In0.53Ga0.47As capacitors with and without an
Al2O3 interface control layer, Appl. Phys. Lett. 97 (2010) 052904-3
 International Centre for Diffraction Data (ICDD) card number 42-1468.
 V. Khranovskyy V, I. Tsiaoussis, L. Hultman L and R. Yakimova, Selective homoepitaxial
growth and luminescent properties of ZnO nanopillars, Nanotechnology 22 (2011) 185603.
 B. Ma, G.K.L. Goh, J. Ma, T.J. White, Growth Kinetics and Cracking of Liquid- Phase-
Deposited Anatase Films, J. Electrochem. Soc. 154 (2007) D557.
 J. J. Brown and F.A. Hummel, Phase Equilibria and Manganese-Activated Luminescence in
the Systems CdO-P2O5 and Zn2P2O7-Cd2P2O7; Summary for the System ZnO-CdO-P2O5, J.
Electrochem. Soc. 111 (1964) 1052–1057.
 V. Khranovskyy, R. Minikayev, S. Trushkin, G. Lashkarev, V. Lazorenko, U. Grossner, W.
Paszkowicz, A. Suchocki, B. G. Svensson, R. Yakimova, Improvement of ZnO thin film properties
by application of ZnO buffer layers, J. Cryst. Growth 308 (2007) 93–98.
 A.R. Kaul, O.Yu. Gorbenko, A.N. Botev, L.I. Burova, MOCVD of pure and Ga-doped
epitaxial ZnO, Superlattices Microstruct. 38 (2005) 272–282.
 L. Xu, L. Shi, X. Li, Effect of TiO2 buffer layer on the structural and optical properties of ZnO
thin films deposited by E-beam evaporation and sol–gel method, Appl. Surf. Sci. 255 (2008) 3230-
 B. P. Zhang, K. Wakatsuki, N. T. Binh, N. Usami, and Y. Segawa, Effects of growth
temperature on the characteristics of ZnO epitaxial films deposited by metalorganic chemical vapor
deposition, Thin Solid Films, 449 (2004) 12-19.
 V.V. Khomyak, M.M. Slyotov, I.I. Shtepliuk, G.V. Lashkarev, O.M. Slyotov, P.D.
Marianchuk, V.V. Kosolovskiy, Annealing effect on the near-band edge emission of ZnO, J. Phys.
Chem. Solids, 74 (2013) 291–297.
 V. Khranovskyy, U. Grossner, V. Lazorenko, G. Lashkarev, B.G. Svensson, R. Yakimova,
Study of annealing influence on electrical and morphological properties of ZnO:Ga thin films
Physica Status Solidi C, 3 (2006) 780-784.
 D.W. Ma, Z.Z. Ye, H.M. Lu, J.Y. Huang, B.H. Zhao, L.P. Zhu, H.J. Zhang, P.M. He,
Sputtering deposited ternary Zn1-xCdxO crystal films on Si(111) substrates, Thin Solid Films 461
(2004) 250– 255
 S. H. Park, T. Hanada, D. C. Oh, T. Minegishi, H. Goto, G. Fujimoto, J. S. Park, I. H. Im, J.
H. Chang, M. W. Cho, T. Yao and K. Inaba, Lattice relaxation mechanism of ZnO thin films grown
on c-Al2O3 substrates by plasma-assisted molecular-beam epitaxy, Appl. Phys. Lett. 91 (2007)
 Z. Ye, D. Ma, J. He, J.Huang, B. Zhao, X. Luo, Z. Xu Structural and photoluminescent
properties of ternary Zn1-xCdxO crystal films grown on Si(1 1 1) substrates, J. Cryst.Growth 256
 G.K. Williamson and W.M. Hall, X-ray line broadening from filed aluminium and wolfram,
Acta Metall. 1 (1953) 22–31.
 B. Williamson, R.C. Smallman, Dislocation densities in some annealed and cold-worked
metals from measurements on the X-ray debye-scherrer spectrum, Philos. Mag. 1 (1956) 34.
 J.Yang, J. Lang, L. Yang, Y. Zhang, D. Wang, H. Fan, H. Liu, Y. Wang, M. Gao, Low
temperature growth and optical properties of ZnO nanorods, J. Alloys Compd. 450 (2008) 521.
 X.Q. Wei, J.Z. Huang, M.Y. Zhang, Y. Du, B.Y. Man, Effects of substrate parameters on
structure and optical properties of ZnO thin films fabricated by pulsed laser deposition, Mater. Sci.
Eng. B 166 (2010) 141–146.
 V. Khranovskyy, A. Ulyashin, G. Lashkarev, B.G. Svensson, R. Yakimova, Morphology,
electrical and optical properties of undoped ZnO layers deposited on silicon substrates by
PEMOCVD , Thin Solid Films 516 (2008) 1396-1400.
 S.R. Haldar, A. Nayak, T.K. Chini, S. Bhuni/ Strong temperature and substrate effect on ZnO
nanorod flower structures in modified chemical vapor condensation growth, Curr. Appl Phys. 10
 K. Sakurai, T.Takagi, T. Kubo, D. Kajita, T.Tanabe, H. Takasu, S. Fujita, S. Fujita, Spatial
composition fluctuations in blue-luminescent ZnCdO semiconductor films grown by molecular
beam epitaxy, J. Cryst. Growth 237 (2002) 514–517.
 A. Teke, Ü. Özgür, S. Doğan, X. Gu, H. Morkoc, B. Nemeth, J. Nause, and H. O. Everitt
Excitonic fine structure and recombination dynamics in single-crystalline ZnO, Phys. Rev. B. 70
 W. F. Yang, R. Chen, B. Liu, G. G. Gurzadyan, L. M. Wong, S. J. Wang, and H. D. Sun,
Surface-Plasmon enhancement of band gap emission from ZnCdO thin films by gold particles,
Appl. Phys. Lett. 97 (2010) 061104.
 B. Guo, Zhizhen Ye, K.S. Wong, Time-resolved photoluminescence study of a ZnO thin film
grown on a (1 0 0) silicon substrate, J. Cryst. Growth, 253 (2003) 252–257.
 T. Koida, S. F. Chichibu, A. Uedono, A. Tsukazaki, M. Kawasaki, T. Sota, and H. Koinuma,
Correlation between the photoluminescence lifetime and defect density in bulk and epitaxial ZnO,
Appl. Phys. Lett. 82 (2003) 532.
W. M. Kwok, A. B. Djurišić, Y. H. Leung, W. K. Chan, and D. L. Phillips, Time-resolved
photoluminescence from ZnO nanostructures, Appl. Phys. Lett. 87 (2005) 223111.
Y. Kawakami, A. Kaneta, K. Omae, A. Shikanai, K. Okamoto, G. Marutsuki, Y. Narukawa, T.
Mukai, and Sg. Fujita, Recombination dynamics in low-dimensional nitride semiconductors, Phys.
Stat. Sol. (b) 240 (2003) 337– 343.
 F. Oba, S. R. Nishitani, S. Isotani, and H. Adachi, I. Tanaka, Energetics of native defects in
ZnO, J. Appl. Phys., 90/2 (2001) 824-828
 Yu. Narukawa, Sh. Saijou, Yo. Kawakami, Sh. Fujita, T. Mukai, and Sh. Nakamura, Radiative
and nonradiative recombination processes in ultraviolet light-emitting diode composed of an
In0.02Ga0.98N active layer, Appl. Phys. Lett. 74 (1999) 558–560.
 S. Chichibu, T. Azuhata, T. Sota, and S. Nakamura, Spontaneous emission of localized
excitons in InGaN single and multiquantum well structures, Appl. Phys. Lett. 69 (1996) 4188.
 Y. Narukawa, Y. Kawakami, M. Funato, Sg. Fujita, and S. Nakamura, Role of self-formed
InGaN quantum dots for exciton localization in the purple laser diode emitting at 420 nm, Appl.
Phys. Lett. 70 (1997) 981.
 Y. Narukawa, Y. Kawakami, Sz. Fujita, Sg. Fujita, and S. Nakamura, Recombination dynamics
of localized excitons in In0.20Ga0.80N-In0.05Ga0.95N multiple quantum wells Phys. Rev. B 55